#------------------------------------------------------------------------------
#$Date: 2022-10-03 17:40:12 +0300 (Mon, 03 Oct 2022) $
#$Revision: 278324 $
#$URL: file:///home/coder/svn-repositories/cod/cif/2/00/08/2000808.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2000808
loop_
_publ_author_name
'Mereiter, K.'
'Preisinger, A.'
_publ_section_title
;
 Structure of Ba₃(AsS₄)₂.7H₂O at 125 K
;
_journal_issue                   6
_journal_name_full               'Acta Crystallographica Section C'
_journal_page_first              984
_journal_page_last               987
_journal_paper_doi               10.1107/S0108270191013938
_journal_volume                  48
_journal_year                    1992
_chemical_formula_sum            'As2 Ba3 H14 O7 S8'
_chemical_formula_weight         944.45
_space_group_IT_number           14
_space_group_name_Hall           '-P 2yn'
_space_group_name_H-M_alt        'P 1 21/n 1'
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_cell_angle_alpha                90
_cell_angle_beta                 97.990(10)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   12.450(2)
_cell_length_b                   12.727(3)
_cell_length_c                   12.694(2)
_cell_volume                     1991.9(7)
_diffrn_radiation_type           Mo
_diffrn_radiation_wavelength     .71069
_exptl_absorpt_coefficient_mu    9.99
_exptl_crystal_density_diffrn    3.149
_exptl_crystal_F_000             1728
_cod_data_source_file            se0081.cif
_cod_data_source_block           se0081a
_cod_original_cell_volume        1991.8(8)
_cod_original_sg_symbol_H-M      'P 21/n'
_cod_database_code               2000808
loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 x,y,z
2 -x+1/2,y+1/2,-z+1/2
3 -x,-y,-z
4 x+1/2,-y+1/2,z+1/2
loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
Ba(1) .165830(10) .262660(10) .123410(10)
Ba(2) .241120(10) .118770(10) .567180(10)
Ba(3) .290400(10) .477370(10) .595830(10)
As(1) .39980(2) .24553(2) .86310(2)
As(2) .41205(2) .25821(2) .37519(2)
S(1) .22868(5) .23960(5) .87542(5)
S(2) .42202(5) .26982(5) .69829(5)
S(3) .46710(5) .09491(5) .91701(5)
S(4) .47909(5) .37480(5) .95437(5)
S(5) .24158(5) .28241(5) .38240(5)
S(6) .43610(5) .25704(5) .21012(5)
S(7) .47025(5) .11722(5) .45913(5)
S(8) .49240(5) .39172(5) .45882(5)
O(1) .12486(16) .05739(17) .23324(17)
O(2) .11547(16) .45101(16) .22192(16)
O(3) .21704(16) -.04919(17) .42256(16)
O(4) .21560(16) .56861(16) .40498(15)
O(5) .10036(16) .05101(16) .71171(16)
O(6) .17508(17) .47125(17) .78448(17)
O(7) .14144(16) .31189(17) .60398(16)
H(1) .0972 .0064 .1807
H(2) .0643 .0944 .2547
H(3) .0836 .5046 .1743
H(4) .0630 .4306 .2668
H(5) .1522 -.0836 .4373
H(6) .1991 -.0080 .3592
H(7) .1479 .6009 .4146
H(8) .2040 .5275 .3410
H(9) .0681 -.0044 .6666
H(10) .0445 .1006 .7214
H(11) .1074 .4942 .7458
H(12) .1642 .4028 .8130
H(13) .0916 .3230 .5401
H(14) .0999 .2982 .6609
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
Ba(1) S(5) 3.3010(10)
Ba(1) S(6) 3.3930(10)
Ba(1) O(1) 3.038(2)
Ba(1) O(2) 2.814(2)
Ba(2) S(2) 3.2400(10)
Ba(2) S(5) 3.1370(10)
Ba(2) S(7) 3.3330(10)
Ba(2) O(3) 2.807(2)
Ba(2) O(5) 2.842(2)
Ba(2) O(7) 2.821(2)
Ba(3) S(2) 3.2810(10)
Ba(3) S(5) 3.6620(10)
Ba(3) S(8) 3.4280(10)
Ba(3) O(4) 2.731(2)
Ba(3) O(6) 2.959(2)
Ba(3) O(7) 2.818(2)
As(1) S(1) 2.1590(10)
As(1) S(2) 2.1700(10)
As(1) S(3) 2.1650(10)
As(1) S(4) 2.1690(10)
As(2) S(5) 2.1590(10)
As(2) S(6) 2.1580(10)
As(2) S(7) 2.1600(10)
As(2) S(8) 2.1720(10)
